Abstract
Severe lattice distortion is a prominent feature of highentropy alloys (HEAs) considered a reason for many of those alloys’ properties. Nevertheless, accurate characterizations of lattice distortion are still scarce to only cover a tiny fraction of HEA’s giant composition space due to the expensive experimental or computational costs. Here we present a physicsinformed statistical model to efficiently produce highthroughput lattice distortion predictions for refractory nondilute/highentropy alloys (RHEAs) in a 10element composition space. The model offers improved accuracy over conventional methods for fast estimates of lattice distortion by making predictions based on physical properties of interatomic bonding rather than atomic size mismatch of pure elements. The modeling of lattice distortion also implements a predictive model for yield strengths of RHEAs validated by various sets of experimental data. Combining our previous model on intrinsic ductility, a data mining design framework is demonstrated for efficient exploration of strong and ductile singlephase RHEAs.
Similar content being viewed by others
Introduction
Highentropy alloys (HEA), or namely the compositionally complex alloys for a broader definition, have attracted a great deal of attention as a promising material solution for addressing the urgent societal goals of reduced carbon emissions and increased energy efficiency. Many HEAs have already been demonstrated to have remarkable yield strengths^{1,2,3,4,5,6,7,8}, great corrosion^{9,10,11,12,13,14} and fatigue resistance^{15,16,17}, reasonable ductility^{3,4,5,6,18,19,20,21,22}, and/or thermal stability^{3,23,24}. More excitingly, the multicomponent chemistry grants HEAs a nearly unlimited design space, making this group of alloys full of potential as revolutionary structural materials for both light weighting and hightemperature applications. The outstanding performances of HEAs are recognized to largely originate from their unique nondilute, multicomponent chemistry and atomic structures at the fundamental level^{25,26,27,28}.
A signature characteristic of the atomic structures of HEAs is severe lattice distortion^{29,30}. In HEAs, multiple types of atoms with different atomic sizes and electronegativities are randomly mixed in a singlecrystal lattice. The size mismatch and charge transfer between individual atoms result in significant variations in interatomic distances and angles. As a result, the atoms cannot reside perfectly on the ideal lattice site, giving rise to a considerable lattice distortion throughout the entire crystal. With respect to the perfect lattice, the distorted lattice of HEAs generates atomic strains that fluctuate from one atom to another, which produces intense interactions with the strain field of dislocations. As a result, every atom in HEAs can actually be considered as a pointpining obstacle to retard dislocation movement, leading to an outstanding solidsolution type strengthening effect^{31,32,33,34,35}. For instance, extremely high yield strengths have been achieved in HEAs by elaborate manipulation of lattice distortion^{4,36,37,38,39}. Additionally, lattice distortion is also recognized to play essential roles in the phase stability^{40,41}, sluggish diffusion^{42,43}, electrical^{44,45}, and thermal conductivities^{45} of HEAs. Therefore, a deep understanding of lattice distortion could assist the design of highperformance HEAs without wandering in the endless compositional space.
Lattice distortion in HEAs can be accurately characterized for individual alloy compositions through various experimental methods, including neutron diffraction, synchrotron Xray diffraction, and highresolution transmission electron microscopy^{4,37,38,46}. Additionally, firstprinciples calculations based on density functional theory (DFT) have been extensively applied to study lattice distortion owing to the accurate description of interatomic bonding. The supercell method based on the special quasirandom structure (SQS)^{47} is widely employed to mimic the multicomponent random mixing in HEAs^{33,47,48,49}. The alloy’s atomic structure at the ground state can be straightforwardly obtained by performing a relaxation calculation. Based on the relaxed structure, lattice distortion can be accurately quantified via a variety of analysis approaches, such as radial or pair distribution function^{50,51}, bond length distribution and fluctuation^{36,49}, local atomic volume^{52}, leastsquare atomic strain^{53}, and mean square average atomic displacement (MSAD)^{33}. Nevertheless, like the experimental approaches, most of the time the DFT calculations were only able to selectively study a small group of discrete alloy compositions due to large computational costs. Apart from the accurate experimental characterization and DFTbased computation, several mathematical models have been proposed for predicting lattice distortion simply according to the alloy composition. However, those models usually oversimplified lattice distortion as the difference in the pureelement atomic size of the constituent elements by assuming that each atom retains its original size even in a complex solidsolution environment. This assumption fails to account for the changes in atomic radii due to charge transfer among constituent atoms, which thus becomes problematic for predicting lattice distortion in the systems containing elements with similar atomic sizes but different electronegativities^{37,54}. The lack of a generally applicable model for rapid and accurate predictions of lattice distortion for arbitrary alloy compositions significantly limits our ability to explore the large design spaces of HEA efficiently.
In the present work, a surrogate model based on physicsinformed statistical learning and training data from firstprinciples calculations is developed to efficiently predict the lattice distortion in the bodycenteredcubic (bcc) refractory HEAs (RHEAs) with compositions arbitrarily varying in chemical space composed of ten elements. The study is centered on RHEAs because they are not studied as comprehensively as the facecenteredcubic (fcc) 3dtransitionmetal HEAs though lattice distortion is indeed found to be significant in individual cases and critically contribute to the mechanical strength^{4,35,36}. The lattice distortion is quantified using the root mean squared atomic displacement (RMSAD), which measures the average displacement of relaxed atoms from their ideal positions in the undistorted crystal lattice^{33,55}. On the basis of physical descriptors that characterize atomic bonds of pure metals and their binary ordered compounds, the developed surrogate model delivers highthroughput predictions of lattice distortion quantified in a way that previously can be only done for individual compositions by costly experiments or firstprinciples calculations. The highthroughput prediction enables a systematic overview of lattice distortion in the alloys with different levels of chemical complexity, from which the physical mechanism of HEA’s unique cocktail effect on lattice distortion is revealed.
Based on the predictions of the lattice distortion model, it is further found that the RMSAD parameter quantitatively correlates with the roomtemperature yield strengths of the bcc refractory alloys in a general linear form. Accordingly, a strengthening model is established to effectively predict yield strengths of RHEAs according to their lattice distortion. Together with our previous surrogate models on intrinsic ductility^{56} and CALculation of PHAse Diagram (CALPHAD)based phase stability prediction, a highthroughput alloy design framework is demonstrated to perform comprehensive screening of potential alloy compositions with a synergy of high strength and good ductility in a large compositional space far from fully explored.
Results and discussion
Initial data exploration
As schematically illustrated in Fig. 1, due to lattice distortion, atoms at equilibrium positions in a solidsolution alloy are locally displaced away from their ideal positions in a perfect, undistorted lattice. A mean squared average of those atomic displacements (i.e., the MSAD) has been demonstrated an accurate quantitative measure of lattice distortion in 3dtransitionmetal HEAs both experimentally and computationally^{33,57,58}. In the present work, the square root of the mean squared atomic displacement (i.e., the RMSAD parameter) is used to quantify lattice distortion because of its strong linear correlation with yield strength^{33,57}. Through a DFT relaxation calculation, the RMSAD parameter for a given alloy composition can be straightforwardly derived as described in the method section in detail. To generate the training and testing data for the development of a surrogate predictive model for lattice distortion, we computed the RMSAD parameters of 215 individual alloy compositions as listed in Supplementary Table 1. Prior to using those DFT data for direct statistical regressions, we first utilized them to perform an initial data exploration, aiming to gain enough physical insights of lattice distortion to better develop the surrogate model. We limited the exploration process to the training dataset, which only contains binary and ternary alloys. As a result, the subsequent development of the surrogate model based on the data exploration is completely blind to the validation and testing datasets (i.e., quaternary and quinary alloys), and those datasets were thus valid to use for testing the model’s ability of extrapolative prediction.
The standard deviation of local atomicbond lengths was naturally considered as a starting point for exploring RMSAD, because an ideal, undistorted bcc lattice would have uniform local bond lengths for every atom, and any displacement of an atom from its ideal lattice site would introduce the variance to the interatomicbond lengths between the displaced atom and its neighbors. In the present work, we calculated the length of every firstnearest neighbor (FNN) atomic bond in the relaxed SQS’s using Voronoitessellation analysis, as implemented in the Pymatgen Python package^{59}, and then derived the standard deviation of the bond lengths (\(\sigma _{{{{\mathrm{SQS}}}}}^L\)) in comparison with the RMSAD parameter obtained for the same structure. A scatter plot shown in Fig. 2a depicts a strong positive correlation between the \(\sigma _{{{{\mathrm{SQS}}}}}^L\) and RMSAD for the alloy samples in the training dataset, with a correlation coefficient, r = 0.94, and significance level, p < 0.001. The correlation indicates that the lattice distortion in solidsolution alloys tightly connects to the length divergence of individual local atomic bonds. In addition, there are two apparent outliers to be off from the correlation displayed in Fig. 2a, which are NbTi_{2} and NbHf_{3}. A common feature of the two alloys is their high content of the group IV element, giving valence electron concentrations (VECs) that are at the lower end of those represented in the training dataset. This trend implies that the dband filling effect may also play a key role to affect the lattice distortion in bcc refractory solidsolution alloys.
Accordingly, a scatter plot of VEC against RMSAD is displayed in Fig. 2b for the alloys in the training dataset. It was found that RMSAD showed a typical dependence on the average filling fraction of the dband. Specifically, the RMSAD parameter becomes lower around VEC of 5.5 e^{−}/atom, which corresponds to an averagely halffilled dband, and becomes higher when the VEC is outside the range of 5.0–6.0 e^{−}/atom, at which the dband deviates from the halffilled state. In addition to this general dband filling dependence, Fig. 2b also highlights an interesting phenomenon that RMSAD can still vary greatly for the alloys with the same VEC. A typical example is the TiRu binary system. As presented in Fig. 2b, although all the three studied TiRu alloys have VECs within the range of 5.0–6.0 e^{−}/atom, they tend to have more severe lattice distortion (i.e., a larger RMSAD), compared to other alloys with the same VECs. It should be noted that the bcc solidsolution phase is metastable for studied TiRu compositions^{60}. The observed severe lattice distortion actually reflects the strong phasetransformation tendency from the disordered solid solution to ordered intermetallic compounds. Another obvious distinction of the studied TiRu alloys from others with similar VECs is that its constituent elements, Ti and Ru, have very different numbers of valence electrons. Considering the strong localization tendency of valence d electrons, one can expect that the local distribution of the d electrons at the TiTi, TiRu, and RuRu atomic bonds in the alloy are inhomogeneous, giving local fluctuations in the VEC. Given this insight, the standard deviation of the number of valence electrons of the constituent elements relative to VEC (\(\sigma ^{{{{\mathrm{VEC}}}}}\)) is also calculated and plotted to against RMSAD in Fig. 2c. As expected, \(\sigma ^{{{{\mathrm{VEC}}}}}\) shows a general positive correlation with RMSAD, suggesting that in addition to the bondlength divergence, the divergence in the dband filling fraction at local atomic bonds, which is induced by the variance of constituent element valences, could also be an important contributor to lattice distortion.
A physically interpretable surrogate model for RMSAD prediction
Although the DFTSQS calculations provide a general approach to assess the lattice distortion of each individual alloy composition by predicting the RMSAD parameter, the relatively large size of SQS supercells make the calculation computationally expensive and consequently, illsuited for highthroughput screening. Therefore, to fully explore the complex compositional space of RHEAs, it is necessary to develop surrogate models for more efficient prediction of RMSAD.
The data exploration discussed above provides a theoretical basis to raise a set of physical descriptors and an interpretable linear model to quantitatively describe RMSAD. As shown in Fig. 2a, the RMSAD parameter displays a strong linear correlation with the standard deviation of the FNN bond lengths in relaxed SQS’s (\(\sigma _{{{{\mathrm{SQS}}}}}^L\)). However, \(\sigma _{{{{\mathrm{SQS}}}}}^L\) cannot be directly used as a descriptor for the prediction of RMSAD because its obtainment requires expensive DFT calculations to relax the SQS for each alloy composition of interest. A surrogate approach is thus needed to efficiently estimate the variance in lengths of FNN atomic bonds in a solidsolution alloy.
As discussed later in the methods section, the FNN atomic bonds in the singleelement bcc and binary B2 crystals can serve as an approximation to those in the solidsolution lattice if only the atomicpair interactions in the FNN shell are considered. We expect that this assumption is particularly reasonable for the transition metal alloy systems as the valence d electrons are strongly localized. As a validation, the lengths of the FNN atomic bonds derived from the DFTrelaxed SQS’s are compared with their respective lengths in the singleelement bcc and binary B2 crystals by showing the histogram of relative deviations in Supplementary Fig. 1. By comparing across a considerable amount of FNN bonds in the SQS’s of 68 binary and ternary alloys, the mean error and root mean square error (RMSE) are only 0.0009 Å and 0.0312 Å (−0.0567% mean relative error and 2.258% root mean square relative error), respectively, which validates our assumption. Therefore, the standard deviation of atomic bond lengths in a solidsolution alloy can be effectively estimated from the lengths of the FNN bonds in the singleelement bcc and binary B2 structures using the bondcounting approach described in the method section. Correspondingly, a descriptor for the bond length standard deviation, \(\sigma _{{{{\mathrm{bcc}}}}/{{{\mathrm{B}}}}2}^L\), is derived. Based on Eq. (6), \(\sigma _{{{{\mathrm{bcc/B}}}}2}^L\) can be easily calculated for any alloy composition of interest without the need to run expensive DFTSQS calculations.
As shown in Fig. 2d, the correlation between the RMSAD and the bondlength standard deviation (\(\sigma _{{{{\mathrm{bcc}}}}/{{{\mathrm{B}}}}2}^L\)) calculated using Eq. (6) is also significant (p < 0.001). On the other hand, significant variability in RMSAD remains unaccounted for by \(\sigma _{{{{\mathrm{bcc}}}}/{{{\mathrm{B}}}}2}^L\) alone as evidenced by an increase in the number of outliers compared to \(\sigma _{{{{\mathrm{SQS}}}}}^L\), suggesting that it is insufficient on its own. The results of data exploration in Fig. 2b, c suggest that the dband filling effect could be another important contributor to lattice distortion in addition to the bondlength standard deviation. Therefore, it is natural to consider VEC as a possible descriptor to explain the discrepancies in the RMSAD vs. \(\sigma _{{{{\mathrm{bcc}}}}/{{{\mathrm{B}}}}2}^L\) correlation, especially given that all the outliers share VECs much lower than those of other samples. To test this hypothesis, the residuals of a linear regression of RMSAD on \(\sigma _{{{{\mathrm{bcc}}}}/{{{\mathrm{B}}}}2}^L\) is plotted to against the VEC of each sample in the training set in Supplementary Fig. 2a, where the residuals show a clear parabolic dependence on VEC with a vertex between VECs of 5 and 6. Based on this observation, we modified VEC into a new descriptor, \(u_{5.7}^{{{{\mathrm{VEC}}}}}\), with the form (VECX)^{2}, where X is a constant tuned to be 5.7 e^{−}/atom by selecting the value that maximizes the correlation coefficient (Pearson’s r) between the transformed feature and RMSAD (Supplementary Fig. 2b). Similarly, another descriptor, \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\), which describes the variance of VEC from 5.7 e^{−}/atom, was created to capture the fluctuation of VEC at different local atomic bonds in the solidsolution lattice. Similar to the feature standard deviation described in Eq. (6), \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\) is calculated as a modified variance of a discrete probability distribution as follows, \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}} = \mathop {\sum }\nolimits x_i\left( {{{{\mathrm{VEC}}}}_i  5.7} \right)^2\). Where x_{i} is the chemical composition of the constituent element, i, and VEC_{i} is its number of valence electrons. As expected, \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\) also shows a strong correlation with RMSAD (Supplementary Fig. 2c).
In addition to VEC, the bimodality of the electronic density of state (DOS) of the dorbitals is also a key factor to determine the dband filling effects^{61}. The localized characteristics of d electrons cause their DOS to display considerable shape features that strongly depend on the lattice structure. For example, a perfect bcctype lattice generally results in a bimodal DOS of the dorbitals. Once the bcc lattice is distorted, such as due to the presence of crystal defects, the shape of the DOS becomes less bimodal^{61}. An extreme situation is that the bcc lattice changes to the fcc/hcp (hexagonalclosepacked) lattice through phase transformation. Correspondingly, the shape of the DOS also changes from bimodal to unimodal. More importantly, the change of bimodality can strongly influence the dbandfilling energy as well as the stability of the crystal lattice when the filling fraction varies. As shown in Fig. 3a, when the dband is about halffilled, which corresponds to a VEC between 5 and 6, a bimodal DOS would have more occupied states far below Fermi Level (E_{f}) and fewer occupied states close E_{f}, compared to that of the unimodal DOS. This trend leads to a more negative bandfilling energy, and correspondingly make the bcc lattice stable. Inversely, when the filling fraction of the dband towards to the edges, a lower band filling energy is expected for the less bimodal DOS, correspondingly stabilizing the non/distortedbcc lattice (Fig. 3b). This principle well explains the effect of dband bimodality on lattice distortion. For instance, if two elements with fewer d electrons (e.g., Ti, Zr, Hf) are forced to form an atomic bond in an undistorted bcc lattice, the DOS of the local dband between them will then have a bimodal shape but a filling fraction near the leftband edge. As a result, the filling energy of the local dband will be high, resulting in a negative effect on the lattice stability. To lower the bandfilling energy and stabilize the bcc lattice, a local lattice distortion is thus necessary to reduce the bimodality of the local dband DOS. In other words, a stronger local lattice distortion shall be expected between two atoms if their atomic bond in the undistorted lattice has a local dband that has a more bimodal DOS and a filling fraction more away from the halffilled state.
The bimodality of a DOS can be quantitatively measured through the Hartigan’s dip test^{61,62}. A completely unimodal DOS corresponds to a test statistic (i.e., the dip value) of 0, while a more bimodal DOS has a larger dip value. In the present work, the average bimodality of the dband DOSs of the FNN atomic bonds (\(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^{{{{\mathrm{dip}}}}}\)) in a bcc solidsolution alloy at the undistorted state is estimated using Eq. (5) based on the bondcounting approach described in the method section. Considering the positive correlation of lattice distortion with both the filling fraction and bimodality of the local dband DOS, we further weigh the two VECassociated descriptors, \(u_{5.7}^{{{{\mathrm{VEC}}}}}\) and \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\)with the bimodality parameter \(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^{{{{\mathrm{dip}}}}}\) for a complete description of the dband effect on lattice distortion. By testing the Pearson’s correlation with RMSAD, the square of \(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^{{{{\mathrm{dip}}}}}\) (i.e., \((u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^{{{{\mathrm{dip}}}}})^2\)) turns to be the optimal weighing factor to result in the largest correlation coefficients.
With the descriptors discussed above, a physically interpretable model is developed to efficiently predict the RMSAD parameter of arbitrary bcc solidsolution alloys within the 10element composition space studied in the present work. The model expresses RMSAD in a linear form with three terms,
where a_{1}, a_{2}, and a_{3} are the fitting coefficients obtained by performing ordinary least squares (OLS) regression with the available DFT data. As shown in Fig. 4a, by only regression with the binary and ternary data, the resulting model can already accurately predict the RMSAD of the quaternary alloys in the validation dataset with an RMSE of 0.012 Å, which is comparable to its training RMSE, 0.015 Å. The regressed values of a_{1}, a_{2}, and a_{3} are summarized in Table 1. Additionally, to confirm the stability and generalization of the model, we reperformed the regression on the data of binary, ternary, and quaternary alloys and tested the correspondingly obtained model with the DFTcalculated RMSAD of quinary alloys. As expected, the values of the fitting coefficients (i.e., a_{1}, a_{2}, and a_{3}) are negligibly varied after additionally including the quaternary data in the regression, indicating the good stability of the proposed linear model. Additionally, as shown in Fig. 4b, the testing performance of the model on the quinary data is also promising, yielding an RMSE of 0.017 Å over 52 testing compositions. The results of Fig. 4 strongly suggest that the proposed linear model well captures the underlying physical mechanism of RMSAD, which grants the model outstanding capability to make accurate extrapolative predictions for multicomponent systems by only training with a finite amount of binary and ternary data.
It is further interesting to point out that a_{1}, a_{2}, and a_{3} all have positive values, which is consistent with the physical motivation of the model. First, a positive a_{1} indicates that a more severe lattice distortion should be expected in an alloy if it has larger deviations in the lengths of local atomic bonds, which is consistent with the observations in Fig. 2a, d. In the previous classical models of lattice distortion, the standard deviation of the atomic radii of pure elements are commonly adopted to describe the variance of atomic bond lengths by assuming atoms are all rigid particles. This assumption fails to consider the bondlength changes due to the possible electron density overlap between heteroelements, which leads to an overestimation on the lattice distortion in some bcc refractory alloys^{37,54}. In the present work, we tackled this problem by using a bondcounting approach (Eqs. (5) and (6) in the methods section). Particularly, the bond length between two heteroelements can be approximated from their binary B2 structure by taking into account the possible charge transfer when forming a bond. Second, a positive value of a_{2} is consistent with our above analysis of the dband effects on lattice distortion; the lattice distortion in an alloy becomes stronger if the average filling fraction of the d orbitals of the alloy is more away from halffilled (i.e., a larger value of \(u_{5.7}^{{{{\mathrm{VEC}}}}}\)) or the shape of the local dorbital DOSs is more bimodal (i.e., a larger value of \(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^{{{{\mathrm{dip}}}}}\)). Third, the positive contribution of VEC standard deviation to lattice distortion is also confirmed by a positive a_{3} coefficient. Overall, the proposed model suggests that the lattice distortion of bcc refractory solidsolution alloys is mainly attributed to two key factors: 1) the significance of the variance in the lengths of local atomic bonds; and 2) the dband effect described by the filling fraction and bimodality of dorbital DOS.
Prediction of yield strength based on the RMSAD parameter
One of the primary motivations behind developing indepth understanding of lattice distortion is its physical correlation with solidsolution strengthening, which consequently provides a possible route to design highstrength HEAs. As discussed in the introduction section, ubiquitous lattice distortion over the crystal lattice could introduce significant atomic strains with random spatial fluctuations, which can elastically interact with the strain field of dislocations and provide a pinning force to retard the dislocation movement. Outstanding yield strengths have been generally achieved in the HEAs with severe lattice distortion^{3,4,63}. The correlation between the lattice distortion and yield strength has also been discussed previously in a few individual alloy systems, including fcc HEAs composed of 3d transition metal elements^{33}, and bcc Nbbased^{35,64} and fcc Nibased solidsolution alloys^{34}.
In spite of the great success of these previous works, the correlation has sofor been only quantitatively confirmed for a few equimolar alloy compositions in rather limited compositional spaces. Our surrogate model of lattice distortion provides an opportunity for performing a more comprehensive assessment in a much broader space, because the model enables a rapid prediction of RMSAD for any given alloy compositions with the studied ten refractory elements. Towards this goal, we have tried to collect an exhaustive set of the roomtemperature experimental yield strength and hardness data from a recent HEA database developed by Citrine Informatics and other literatures^{2,19,20,65,66,67,68,69,70,71,72,73,74,75,76,77,78,79,80,81,82,83,84,85,86,87,88,89,90,91,92,93,94,95}. In total 83 yield strength and 28 hardness data were collected, which covered 66 individual compositions (30 equiatomic, and 33 nonequiatiomic cases), ranging from quaternary to senary systems (Supplementary Table 2). The data collection is limited to ascast and annealed alloys, so the strengthening effects due to processing such as grain refinement and strain hardening can be minimized. The detail of our datacollection process is described in the methods section. Then, regarding each of the experimental data, the surrogate model is employed to predict RMSAD according to the alloy composition in order to investigate the potential correlation between the lattice distortion and yield strength.
A modified theory of solidsolution strengthening for random alloys has been recently developed by Maresca and Curtin^{28}. The theory expresses the athermal yield strength (τ_{Y}) of a bcc solidsolution alloy as,
In the equation, α is the dislocation linetension parameter, which is a constant for a given type of dislocation, and \(\left( {\frac{{1 + v}}{{1  v}}} \right)^{\frac{4}{3}}\) is a term of elastic anisotropy calculated by the Poisson’s ratio (v), which is usually insensitive to the variation of alloy compositions^{96}. From the equation, one can consider the variation of the athermal yield strength with alloy composition is dictated by three parts of contributions, the isotropic shear modulus of the alloy, μ, an effective parameter describing the gradient of dislocation stress field, f^{τ}, and the volume misfit quantity, \(\frac{{\mathop {\sum }\nolimits_n c_n\Delta V_n^2}}{{b^6}}\), which is actually closely related to the δ parameter, a commonlyused parameter to describe lattice distortion based on the mismatch of atomic radii. Recently, the volumemisfit quantity has also been found to be strongly correlated with the RMSAD parameter in several HEA systems^{55}, correspondingly evidencing the correlation of the yield strength with lattice distortion.
Therefore, inspired by Eq. (2) above, here we propose a simplified linear expression based on RMSAD to effectively model and predict the roomtemperature yield strength of bcc refractory HEAs, which can be written as,
where μ is still the isotropic shear modulus, γ_{USF} is the average unstable stacking fault (USF) energy of the {110} plane of the alloy, and a is a constant coefficient, which should be universal to different alloy compositions and systems. The derivation of Eq. (3) is based on the three main contributions to yield strength in Eq. (2), where we use RMSAD to parameterize the local atomic misfit strain generated by lattice distortion and use the USF energy (γ_{USF}) to substitute f^{τ} to reflect the gradient of the dislocationstress field. This is because the derivation of f^{τ} is usually a complex process involving extensive data fitting, and in the meanwhile, the gradient of the dislocationstress field should be generally proportional to the width of the dislocation core, which essentially relates to the USF energy according to the PeierlsNabarro model^{96}. Moreover, it is noteworthy that the three parameters, μ, γ_{USF}, and RMSAD, in Eq. (3) at a given alloy composition can be respectively predicted using Vegard’s law^{97,98}, a statistical learning model developed by us previously^{56}, and the present lattice distortion model, without requiring performing any additional timeconsuming calculations. Therefore, Eq. (3) naturally offers a highthroughput prediction approach of yield strength for efficient screening over large compositional spaces.
To validate Eq. (3), experimental yield strength data is normalized by the isotropic shear modulus and USF energy to evaluate its linear dependence on RMSAD. As shown in Fig. 5a, a linear relationship is observed between the normalized yield strength, denoting as \(\tau _{{{\mathrm{Y}}}}/(\mu \gamma _{{{{\mathrm{USF}}}}})\), and RMSAD, giving an R^{2} value as high as 0.94. Additionally, the value of the constant, a, in Eq. (3) can be easily obtained via an OLS regression of \(\tau _{{{\mathrm{Y}}}}/(\mu \gamma _{{{{\mathrm{USF}}}}})\) on RMSAD, which is 0.29 Å/eV. An RMSE of 135 MPa was obtained by comparing the predicted yield strength predicted with the experimental truth. Additionally, it is well known that the hardness of most alloys shows a linear dependence on yield strength in general. Therefore, Eq. (3) should also be capable to model the hardness of bcc refractory HEAs, if it truly sketches the underlying physics of solidsolution strengthening. As expected, a clear linear relationship is also observed between the normalized hardness, \(HV/\left( {\mu \gamma _{{{{\mathrm{USF}}}}}} \right)\), and RMSAD, returning a RMSE of prediction as small as 29.5 HV (Fig. 5b).
Data mining and interpretation
Based on the developed surrogate models, a systematic data mining over massive alloy compositions is performed to uncover the physical relations of lattice distortion to phase stability, strength, and ductility of RHEAs. First, the distribution of lattice distortion in bcc refractory alloys is mapped in a compositional space composed of ten major RHEA elements. Second, with the mapping results of lattice distortion, the roomtemperature yield strengths of those mapped compositions are also predicted, using Eq. (3). Third, the predicted yield strength is leveraged with a previously developed ductility model^{56} and the CALPHAD approach^{99} to validate an integrated computational framework for the datadriven design of RHEAs with high strength and good ductility.
Systematic mapping of lattice distortion
Mapping of lattice distortion is performed for various binary, ternary, quaternary, and quinary alloys in a vast compositional space consisting of ten different elements, namely Ti, Zr, Hf, V, Nb, Ta, Mo, W, Re, and Ru. Compositions considered are limited such that every individual element composes between 10 and 60 atomic percent (at%) to maintain focus on the concentrated, highentropy region of the compositional space. For a homogenous sampling, the binary, ternary, and quaternary alloys are assessed at 5 at% compositional intervals with each element while a 10 at% interval is applied to the quinary alloys. As such, a total of 76,816 compositions are investigated. Of those, 140 compositions are binary alloys; 5208 are ternary; 36,400 are quaternary; and 35,068 are quinary. At each mapped composition, we also utilize the CALPHAD approach^{99} to evaluate the phase stability of the singlephase bcc solid solution at 800 °C, which is a common temperature used for the homogenization processing of RHEAs. After the phasestability evaluation, 5916 compositions are found to result in singlephase bcc solid solutions at 800 °C. Among them, 71 are binary; 1989 are ternary; 2012 are quaternary; and 1844 are quinary.
The mapping results of lattice distortion are shown in Fig. 6a, b where relative frequency histograms showing the distribution of RMSAD for all the screened alloy compositions and those possessing a single bcc phase at 800 °C, respectively. The compositions are grouped into binary/ternary (low/medium entropy) and quaternary/quinary (high entropy) categories to highlight the effect from the number of component elements, i.e., the cocktail effect of HEAs. In Fig. 6a, it can be seen that the RMSAD distributions are nearly identical between the binary/ternary and the quaternary/quinary groups. The mean values of the distributions are also similar, which are 0.1544 Å for the low/mediumentropy alloys and 0.1573 Å for the highentropy alloys. However, when the solidsolution phase stability is considered, obvious difference is observed in the RMSAD distributions between the low/mediumentropy and highentropy alloys. As presented in Fig. 6b, with the singlephase constraint, the RMSAD distribution of the low/mediumentropy group is biased towards the compositions with less lattice distortion. This feature is also evidenced by the increased skewness, which more than doubled (0.70 vs. 1.92) and reduced distribution mean (0.1544 vs. 0.0974 Å). In contrast, the distribution of RMSAD for the highentropy group (quaternary/quinary alloys) does not show significant bias after applying the phasestability restriction, which still holds a mean RMSAD as high as 0.1502 Å and a weak skewness. Comparing the results of Fig. 6a, b suggests that while highly distorted binary and ternary bcc solidsolution alloys are predicted to be possible, a majority of them cannot remain thermodynamically stable at typical processing temperatures. On the other hand, the quaternary and quinary alloys with severe lattice distortions are likely to be stabilized by the increased configurational entropy from the inclusion of multiple principal elements. There has been an enduring debate whether the severe lattice distortion is a feature unique to HEAs or it can be generally exiting in any kind of solidsolution alloys regardless compositional complexity^{100}. The present observation clearly evidences the importance of compositional complexity in preserving solidsolution alloys with severe lattice distortion from phase decomposition.
To uncover the mechanism of the HEA’s cocktail effect on lattice distortion, the singlephasealloy compositions with a RMSAD larger than 0.15 Å are collected for a further investigation, as marked by the red box in Fig. 6b. Here, 0.15 Å is chosen as an indicator for severe lattice distortion, as it represents the 84th percentile of the binary/ternary distribution and the 58th percentile of the quaternary/quinary distribution. In this collective dataset, a comparison between the binary/ternary and quaternary/quinary alloys could clearly elucidate the effects of compositional complexity on severe lattice distortion. According to Eq. (1), a higher degree of lattice distortion can be achieved in an alloy that has a larger deviation in local atomic bond lengths (\(\sigma _{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^L\) in Eq. (1)), a VEC more away from 5.7 e^{−}/atom (\(u_{5.7}^{{{{\mathrm{VEC}}}}}\) in Eq. (1)), and/or a large variability of the number of valance electrons (\(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\) in Eq. (1)) among the constituent elements. The distributions of the \(\sigma _{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^L\), \(u_{5.7}^{{{{\mathrm{VEC}}}}}\), and \(\sigma _{5.7}^{{{{\mathrm{VEC}}}}}\) parameters in the binary/ternary and quaternary/quinary alloys with RMSAD > 0.15 Å are visualized via boxplots, as exhibited in Fig. 6c, d, and e, respectively. It is interesting to note that the quaternary/quinary alloys generally have a larger \(\sigma _{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^L\) than the binary/ternary alloys, but vice versa for the \(u_{5.7}^{VEC}\) parameter. Also, the aforementioned differences are demonstrated to be statistically significant via Welch’s ttests^{101}. This observation suggests that the severe lattice distortion in the quaternary/quinary alloys is more attributed to the deviations in local atomic bond lengths of the constituent elements. However, significant differences in the valences and atomic volumes of the constituent element in a solidsolution phase also leads to a strong driving force for phase decomposition, according to the classic HumeRothery rule. Thanks to the multicomponent chemistry, such a driving force in the quaternary and quinary alloys could be balanced by the stabilization effect induced by the increased configurational entropy. As a result, those alloys can still remain as a singlephase solid solution while bearing a large lattice distortion. On the other hand, it is understandable that the severe lattice distortion in the binary and ternary alloys is more associated with a larger \(u_{5.7}^{{{{\mathrm{VEC}}}}}\) parameter (Fig. 6d), since too large \(\sigma _{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^L\) would introduce phase decomposition, which cannot be sufficiently balanced by the entropy stabilization effect. In fact, the \(u_{5.7}^{{{{\mathrm{VEC}}}}}\) parameter cannot be too large either because the bcc lattice structure becomes unstable for a transitionmetal alloy if its d orbital band is away from the halffilled state^{102}. Therefore, a majority of screened binary and ternary alloys with severe lattice distortion are thermodynamically unstable.
Lattice distortion induced solid solution strengthening
With the results of the RMSAD screening above, we could further evaluate how the yield strengths of the bcc refractory alloys distribute across a large compositional space using the developed strengthening model (Eq. (3)). Here we restrict the yieldstrength prediction to the same alloy compositions in Fig. 6b, which are predicted to be stable as a single bcc solidsolution phase at 800 °C. The compositions with RMSAD less than 0.01 Å, however, are omitted. It is important to note that this exclusion would only disproportionately affect a select few dilute compositions in the MoW binary series, which tend to exhibit low lattice distortion and yet could potentially still be strong due to a high lattice friction stress, as reflected by their shear moduli (Supplementary Table 3). The predicted yield strengths are visualized as distribution histograms to reveal the difference between the binary/ternary and quaternary/quinary alloys. As shown in Fig. 7a, the quaternary/quinary alloys generally possess a higher yield strength and a narrower distribution than those of the binary/ternary alloys. The higher average strength of the quaternary/quinary alloys is likely to be a benefit of higher levels of lattice distortions in those alloys (Fig. 6b), which contributes positively to yield strength according to Eq. (3). Additionally, in our strengthening model, the yield strength of a bcc refractory alloy is also proportional to its shear modulus and USF energy, which are two material features showing strong dependences on VEC. As exhibited in Supplementary Fig. 3, an alloy with a lower VEC that is away from a halffilled d band state generally has a smaller μ and γ_{USF}. Therefore, to achieve a high yield strength in an alloy would require it to have a large RMSAD and meanwhile not a too small VEC. This combination of features is more possible to achieve in the quaternary/quinary alloys due to the entropystabilization effect.
The potentials of RHEAs for light weighting applications are also evaluated through a prediction of specific strength, which is achieved by combining the yield strength data obtained above with a latticeparameter model developed in our recent work for the prediction of theoretical density^{103}. The predicted specific strengths are also overviewed, using the distribution histograms, as shown in Fig. 7b. It is exciting to note that the HEAs also averagely yield higher specific strengths than the alloys with low/medium configurational entropies. The results of Fig. 7 here suggest that more opportunities of lightweight, highstrength alloy compositions shall be expected by increasing the number of components through the “highentropy” design strategy.
Datadriven design of highperformance RHEAs
The current screening model for alloy’s yield strength can be seamlessly integrated with a ductility assessment model developed in our previous work for a datadriven exploration of strong and ductile bcc refractory alloys. Taking alloy composition as input, the ductility model yields rapid prediction for a socalled D parameter, which is defined as the ratio between the surface energy of a crack fracture plane and unstable stacking fault energy of the common dislocationslip plane. The magnitude of the D parameter physically reflects the likelihood of an alloy to be intrinsically ductile, based on the Rice fracture mechanics^{104}. More importantly, the D parameter of RHEAs has been demonstrated to positively correlate with the compression fracture strains measured experimentally, which makes it an effective indictor to assess alloy’s ductility^{56}. A combination of the strength and ductility models with the CALPHADbased assessment of phase stability forms a datadriven design framework that is powerful for performing massive searches in a vast design space for promising alloy compositions with the enhanced ductility and strength. Figure 8a shows the flow chart of the framework. With an input alloy composition, the CALPHADbased thermodynamic assessment is first carried out to check whether the bcc solid solution can be stable as a single phase at a given processing temperature. If yes, the strength and ductility models are sequentially applied to assess the mechanical properties.
As a demonstration, we applied this framework to the same composition dataset used for our latticedistortion mapping, which contains 76,816 compositions homogenously sampling all the binary, ternary, quaternary, and quinary systems in the 10component compositional space. The results are displayed by an Ashby plot of the strengthductility combination in Fig. 8b. Positions of some experimentallystudied RHEAs^{2,19,65,67,68,70,71,72,73,74,75,77,78,80,82,83,84,85,86,87,88,89,90,91,92,93,94,95,105} are also highlighted to manifest the potential area to explore. As shown in Fig. 8b, despite a weak trend of the typical strengthductility tradeoff, the quite dispersed distribution between yield strength and the D parameter illuminates a range of RHEAs that can possess a good combination of strength and ductility. If we consider the alloys with a D parameter larger than 3.3 being potentially ductile, as it generally corresponds to a compression failure strain greater than 40%, there are still a substantial proportion of alloy compositions (marked by a dashed box) could have yield strength greater than 1 GPa but are not fully experimentally explored yet. A recently discovered RHEA, HfTaTiZr, falls in this window, which was indeed measured to have a yield strength about 1.5 GPa and be ductile in tension deformation with limited plasticity, in a good agreement with the present prediction^{67}. Additionally, the alloy’s ductility was found to be significantly improved via proper heattreatment processing^{106}. Furthermore, the scattered distribution of the experimentally reported equimolar alloys in Fig. 8b indicates that maximizing configurational entropy may not always be an optimal design strategy for HEAs and there could be considerable spaces to tune alloy compositions for the improved strength and ductility combination relative to the currently known RHEAs.
Several practical insights are also derived from the current screening, which may enlighten the future design of RHEAs. VEC is unsurprisingly found to be quite influential for both yield strength and ductility (i.e., D parameter). The yield strength and D parameter of the screened alloys is plotted against their VEC in Fig. 8c, d, respectively, with data points color coded corresponding with RMSAD. As shown in Fig. 8c, the yield strength seems to peak at two VEC values, 4.7 and 5.5 e^{−}/atom, respectively. As discussed in Eq. (3), the yield strength is a function of RMSAD, μ, and γ_{USF}. The relation between RMSAD and VEC is discussed in Fig. 2b with lower VECs corresponding with higher RMSAD. When plotted as a function of VEC (Supplementary Fig. 3), μ, and γ_{USF} show a positive correlation with VEC. Based on these observations, The peak at 4.7 e^{−}/atom is attributed to increased lattice distortion and the peak at 5.5 e^{−}/atom is more likely to correspond to higher μ, and γ_{USF.} On the other hand, the D parameter shows a negative dependence on VEC in general, which means that the alloys with larger VEC are likely have poor ductility due to a smaller D parameter. Particularly, regarding the alloys near the yield strength peak with VEC around 5.5 e^{}/atom, their D parameter is only about 2, which is a value exhibited by the alloys showing brittle deformation behaviors^{56}. Therefore, a good balance between the strength and ductility may be achieved by tuning the alloy’s VEC to be around 4.7 e^{−}/atom. Furthermore, the lattice distortion also positively affects both the strength and ductility. For example, as shown in Fig. 8d, alloys with a larger RMSAD generally have a larger D parameter. Also, at a certain level of VEC, increasing the alloy’s RMSAD leads to a further enhancement of the yield strength, as shown by the colormap in Fig. 8c. These observations suggest that a good blend of strength and ductility can be expected if the alloy is designed to have a VEC close to 4.7 e^{}/atom and constitute elements that having large variances in their number of valence electrons and bcc/B2 bond lengths to maximize the lattice distortion (i.e., RMSAD).
In summary, a statistical surrogate model was developed to efficiently predict lattice distortion in bcc refractory nondilute, highentropy solid solution alloys with ten constituent elements: Ti, Zr, Hf, V, Nb, Ta, Mo, W, Re, and Ru. The lattice distortion quantified by the RMSAD parameter was previously only obtained for a few individual alloys by costly experiments or calculations but can now be rapidly predicted by the developed model in a highthroughput manner simply according to alloy composition. Unlike the conventional models based on atomic size mismatch of pure elements, the present model uses descriptors that characterize the length and electronic structure of interatomic bonds in solidsolution alloys for a more accurate description of lattice distortion. With physicsinformed statistical learning, the model exhibits a promising capability to make reliable extrapolative predictions for the multicomponent alloy compositions outside the training data range. Moreover, a strong correlation between the lattice distortion and the roomtemperature yield strength is revealed in bcc RHEAs. Accordingly, a surrogate model enlightened by the recent solidsolution strengthening theory^{28} is proposed for rapid prediction of yield strength of RHEAs simply according to their compositions.
The developed surrogate models are applied to screen over a massive amount of alloy compositions to systematically investigate the compositional dependence of lattice distortion and yield strength in RHEAs. The multicomponent nature (i.e., cocktail effect) of RHEAs is revealed to play a critical role in preventing the highly distorted solidsolution lattice from phase transformation. As a result, severe lattice distortion is found to generally be more achievable in the alloys with higher chemical complexity due to increased configurational entropy. The increased level of lattice distortion also benefits RHEAs to generally have a higher strength than their binary and ternary counterparts. Integration of the developed models with a model of intrinsic ductility^{56} and phase stability assessment based on the CAPHAD approach enables an alloy design platform for highthroughput search of highperformance RHEAs in a large compositional space that is far from being fully explored. The highthroughput search illuminates a range of previously unexplored chemical compositions promising for achieving a singlephase RHEAs with a combination of high strength (>1 GPa) and reasonable ductility. The present work demonstrates a promising route to combine physical principles with statistical approaches for developing efficient surrogate models to accelerate the pace of HEAs’ design and development, especially for those with nonequimolar compositions.
Method
Details of DFT calculations
In the present work, DFT calculations were performed, using the projector augmented wave method^{107} with the exchangecorrelation functional depicted by the general gradient approximation from Perdew, Burke, and Ernzerhof (GGAPBE)^{108}, as implemented in the Vienna abinitio simulation package (VASP)^{109}. The calculation parameters used were the same as those employed in our previous work^{56} with a planewave basis energy cutoff of 400 eV, firstorder Methfessel Paxton smearing of 0.2 eV, and using kpoint grids generated by the VASP’s automatic meshing scheme with an R_{k} length of 30 Å. An Energy convergence criterion of 10^{−6} eV was used for electronic selfconsistency cycles. The atomic structural relaxations were performed by minimizing the atomic forces to be smaller than 0.001 eV/Å. The aforementioned settings of the kpoint density and smearing width were validated by convergence test calculations in our previous work^{56}. The supercells used for DFT calculations were constructed, using the SQS approach to approximate the chemical disorder in solidsolution alloys^{47}. For binary, ternary, and quaternary alloy compositions, the generated SQSs contains 72 atoms, and 120atom SQSs were employed for quinary compositions. Overall, as listed in Supplementary Table 1, the relaxed atomic structures of 69 binary, 36 ternary, 64 quaternary, and 52 quinary bcc refractory alloys were calculated from a compositional space comprised of 10 group IV–VIII elements, including Ti, Zr, Hf, V, Nb, Ta, Mo, W, Re, and Ru. Among the DFT results, 106 of the compositions were adopted from our previous work^{56}.
Scrutiny of bcctoω phase transformation in training data
A bccbased SQS for refractory alloys with low VECs could be dynamically unstable and transform into a lattice closer to the crystal structure of the ω phase after relaxation^{40,41,110}. To ensure that no ωlike structures were included in the training data, an approach developed be Ikeda et al. ^{41} was used. The bcctoω transformation has the martensitic nature and can be caused by atomic shuffling of twothird atoms in the bcc lattice along a \(111_{{{{\mathrm{bcc}}}}}\) direction. Therefore, a SQS of a multicomponent alloy can be considered as being “ω like” if the atomic displacements caused by relaxation display a preference for a particular \(111_{{{{\mathrm{bcc}}}}}\) direction whereas there should be no significant preference if the bcc symmetry is preserved^{41}. The preference can be quantified through a fourstep analysis. First, the atomic displacement of each atom in the supercell is projected along four distinct \(\left[ {111} \right]_{{{{\mathrm{bcc}}}}},\left[ {1\bar 1\bar 1} \right]_{{{{\mathrm{bcc}}}}},\left[ {\bar 11\bar 1} \right]_{{{{\mathrm{bcc}}}}}\) and \(\left[ {\bar 1\bar 11} \right]_{{{{\mathrm{bcc}}}}}\) directions, respectively. Second, the projection magnitude for each \(111_{{{{\mathrm{bcc}}}}}\) direction is averaged over all the atoms in the supercell. Third, the average projection magnitudes along different \(111_{{{{\mathrm{bcc}}}}}\) directions are sorted based on their values. Fourth, a structural descriptor is defined by taking the difference between the largest projection magnitude (p_{1}) and second largest projection magnitude (p_{2}), i.e., p_{1}–p_{2}. A relaxed SQS is considered as being “ω like” if p_{1}–p_{2} is larger than a threshold value, 0.04c_{ω}, where c_{ω} is the lattice parameter of the c axis of a perfect ω crystal which is calculated as a function of the bcc lattice parameter (a_{bcc}) with the relationship: \(c_{\upomega} = \frac{{\sqrt 3 }}{2}a_{{{{\mathrm{bcc}}}}}\). If p_{1}–p_{2} is smaller than 0.04c_{ω}, the bcc symmetry is preserved. By implementing Ikeda’s method, we found that concerning the SQSs used in the present work no structures exceeded this threshold. The calculated p_{1}p_{2} of each SQS is shown in Supplementary Fig. 4. In addition, NbTi_{3} was found to be an outlier relative to the other compositions and was thus removed from subsequent training process as a precautionary measure.
RMSAD parameter
In the present work, the RMSAD parameter was derived from DFT relaxation calculations. Specifically, the RMSAD parameter was calculated by taking the rootmean square average of the Euclidian distances between atomic positions in the relaxed SQS supercell and their corresponding ideal positions in the perfect bcc lattice, which can be expressed as,
where n is the number of atoms in the supercell, \(x_i^{{{{\mathrm{ideal}}}}}\) is the ideal lattice site for atom, i, and \(x_i^{{{{\mathrm{real}}}}}\) is the DFT relaxed position of atom, i. Since the volume of the supercell can also change after relaxation, the ideal position of each atom was attained by scaling the initially unrelaxed supercell to have the same atomic volume as the relaxed one. The Euclidian distance was then calculated in Cartesian coordinates. As such, the calculated Euclidian distance should only reflect the atomicposition deviation due to the local lattice distortion rather than that caused by the change in the volume of the supercell after relaxation.
Physicsinformed descriptors
The selection of the physical feature to construct descriptors was driven by a data exploration described in the result section. It was found that lattice distortion was largely determined by interatomicbonding characteristics like the first nearest neighbor (FNN) bond length and valence electron concentration (VEC) and their variations due to the local chemistry fluctuation caused by random mixing. Therefore, other than VEC, which has a simple derivation, the rest of descriptors were constructed using a bondcountingbased method developed in our previous work, by which the physical characteristics of interatomic bonds in a random alloy can be effectively integrated with its composition^{56}.
According to the bondcounting method^{111,112}, a bulk property of an alloy, such as the cohesive energy, can be approximated as a summation of the individual contributions from each atomic bond in the alloy. In random alloys, the probability of finding an interatomic bond between two constituent elements, i and j, should be statistically equal to the product of the concentration of i and j. Therefore, the summation of individual bond contribution can be considered as a weighted average over different i–j bonds in the alloy, and the weighting factor is the presence probability of each type of i–j bonds. Accordingly, the descriptor can be written as,
where x_{i} and x_{j} are the chemical compositions of elements, i and j, respectively, which are among the 10 refractory elements studied in the present work (i.e., Ti, Zr, Hf, V, Nb, Ta, Mo, W, Re, and Ru). \(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^p\)is a descriptor based on an interatomicbonding feature, p, which has a value of p_{i,j} for the i–j type of atomic bond. Clearly, all values of p_{i,j} can be summarized as a 10 × 10 matrix in which each component stands for a pair permutation between the ten alloying elements. Additionally, to reflect the fluctuations in local atomic environment, the standard deviation of \(u_{{{{\mathrm{B}}}}2/{{{\mathrm{bcc}}}}}^p\) is also taken as a descriptor with an expression as,
To derive the values of p_{i,j} is not trivial. Assuming that the atomic interactions between the atoms as FNN are much stronger than others, we could apply the physical properties of a group of singleelement bcc and ordered binary B2 structures as the bond feature parameter. For example, if we consider the FNN bond length as a bondfeature parameter, its p_{i,i} component thus to be the length of the FNN ii bond in the singleelement bcc structure composed of element, i, while the p_{i,j} and p_{j,i} components are the FNN bond lengths of the binary B2 structure composed of elements, i and j. This assumption is valid because the only type of the FNN atomic bond in a bcc crystal purely comprised of element, i, is the ii bond along the <111> direction, and the only type of the FNN bond in the binary B2 structure composed of elements, i and j, is the i–j bond, as illustrated in Fig. 9. Since there are only two atoms in the unit cell of the singleelement bcc and ordered binary B2 structures, DFT calculations can be easily applied to these structures to predict the values of p_{i,j} without demanding extensive calculations. In the present work, we derived two types of bondfeature parameters from the DFT calculations, which are the FNN bond length (L) and an electronic structure parameter (dip) measuring the bimodality of the local DOS of the d orbitals in the bcc/B2 structures. The dip parameter was designed to account for the nuance of the dband filling effects in bcc transition metals beyond VEC, and demonstrated to great success capturing the effects of interatomic bonding on defect energetics of refractory alloys in our previous work^{56,61}.
Data splitting and statistical regression
Due to the high computational cost, the DFTSQS calculations were only able to generate a finite amount of RMSAD data for 215 individual alloy compositions, which is only a tiny fraction of the full composition space studied in the present work. Therefore, to wisely leverage this small set of DFT data for reliable extrapolative predictions, we did not randomly split them into training and testing datasets. Instead, the obtained DFT data were split into three datasets based on the chemical complexity for training, validation, and testing. Specifically, only the data of binary and ternary alloys were used as training data, quaternary ones as the validation data to determine the best descriptors, and quinary ones were reserved exclusively for a final testing to examine the regression stability of the finalized model and its prediction ability for unseen compositions. This datasplitting strategy allows us to maximally test the prediction capability of the built surrogate models for extrapolative exploration of multicomponent alloy compositions not covered by the training set. Based on the developed descriptors, a modified OLS regression process was employed to develop a predictive model for the lattice distortion (i.e., the RMSAD parameter) in refractory solidsolution alloys. Specifically, the model was constructed piecewise, starting with the descriptors with the strongest correlation, and additional descriptors were sequentially added until no significant improvement in the prediction performance can be achieved.
Collection of the experimental strength data of RHEAs
To explore the deep connection between the lattice distortion and solidsolution strengthening in refractory HEAs, a set of experimental yieldstrength and hardness data were collected from a HEA database recently developed by Citrine Informatics and other literatures^{2,19,20,65,66,67,68,69,70,71,72,73,74,75,76,77,78,79,80,81,82,83,84,85,86,87,88,89,90,91,92,93,94,95}. Specifically, data points were filtered to collect the measurements made at room temperature on bcc singlephase HEAs with constituent elements among the ones studied in the present work. The collection is limited to ascast and annealed alloys to minimize the extrinsic strengthening effects due to processing such as strain hardening and grain refinement and to compression yield strengths because of a relative lack of tensile tested data. Overall, 83 yieldstrength and 28 hardness data were collected, which covered 66 individual alloy compositions, ranging from quaternary to senary systems, as summarized in Supplementary Table 2. For each of the assessed experimental data, its corresponding RMSAD parameter is predicted by the surrogate model developed in the present work for exploring the correlation between lattice distortion and yield strength.
Data availability
All the data associated with the findings of this work is available to the public through an openaccess repository, GitHub (https://github.com/tandocca/LatticeDistortion) as well as in the supplementary information file associated with this manuscript.
Code availability
All the code associated with the findings of this work is available to the public through an openaccess repository, GitHub (https://github.com/tandocca/LatticeDistortion).
References
Lee, C. et al. Strength can be controlled by edge dislocations in refractory highentropy alloys. Nat. Commun. 12, 1–8 (2021).
Zhang, Y., Yang, X. & Liaw, P. K. Alloy design and properties optimization of highentropy alloys. Jom 64, 830–838 (2012).
Zou, Y., Ma, H. & Spolenak, R. Ultrastrong ductile and stable highentropy alloys at small scales. Nat. Commun. 6, 1–8 (2015).
Lee, C. et al. Lattice‐distortion‐enhanced yield strength in a refractory high‐entropy alloy. Adv. Mater. 32, 2004029 (2020).
Pan, Q. et al. Gradient cell–structured highentropy alloy with exceptional strength and ductility. Science 374, 984–989 (2021).
Yang, T. et al. Multicomponent intermetallic nanoparticles and superb mechanical behaviors of complex alloys. Science 362, 933–937 (2018).
Fu, Z. et al. A highentropy alloy with hierarchical nanoprecipitates and ultrahigh strength. Sci. Adv. 4, eaat8712 (2018).
Feng, R. et al. Superior high‐temperature strength in a supersaturated refractory high‐entropy alloy. Adv. Mater. 33, 2102401 (2021).
Qiu, X.W., Zhang, Y.P., He, L. & Liu, C.G. Microstructure and corrosion resistance of AlCrFeCuCo high entropy alloy. J. Alloy. Compd. 549, 195–199 (2013).
Qiu, Y., Thomas, S., Gibson, M. A., Fraser, H. L. & Birbilis, N. Corrosion of high entropy alloys. NPJ Mater. Degrad. 1, 1–18 (2017).
Shi, Y., Yang, B. & Liaw, P. K. Corrosionresistant highentropy alloys: a review. Metals 7, 43 (2017).
Chou, Y. L., Yeh, J. W. & Shih, H. C. The effect of molybdenum on the corrosion behaviour of the highentropy alloys Co1. 5CrFeNi1. 5Ti0. 5Mox in aqueous environments. Corros. Sci. 52, 2571–2581 (2010).
Mao, X. et al. Microstructure and corrosion performance of Al0. 5FeCoNiCrMn coating prepared by plasma spraying mechanically alloyed powders. Surf. Eng. 38, 383–392 (2022).
Wang, C. et al. Chloride corrosion property evolution of CrMnFeCoNi highentropy alloy coating. Mater. Sci. Technol. 38, 1418–1424 (2022).
Chen, P. et al. Fatigue behavior of highentropy alloys: a review. Sci. China Technol. Sci. 61, 168–178 (2018).
Hemphill, M. A. et al. Fatigue behavior of Al0. 5CoCrCuFeNi high entropy alloys. Acta Mater. 60, 5723–5734 (2012).
Li, W., Chen, S. & Liaw, P. K. Discovery and design of fatigueresistant highentropy alloys. Scr. Mater. 187, 68–75 (2020).
Li, P., Wang, A. & Liu, C. T. A ductile high entropy alloy with attractive magnetic properties. J. Alloy. Compd. 694, 55–60 (2017).
Juan, C.C. et al. Solution strengthening of ductile refractory HfMoxNbTaTiZr highentropy alloys. Mater. Lett. 175, 284–287 (2016).
Sheikh, S. et al. Alloy design for intrinsically ductile refractory highentropy alloys. J. Appl. Phys. 120, 164902 (2016).
Chen, R. et al. Composition design of high entropy alloys using the valence electron concentration to balance strength and ductility. Acta Mater. 144, 129–137 (2018).
Wei, S. et al. Naturalmixing guided design of refractory highentropy alloys with ascast tensile ductility. Nat. Mater. 19, 1175–1181 (2020).
LaurentBrocq, M. et al. Insights into the phase diagram of the CrMnFeCoNi high entropy alloy. Acta Mater. 88, 355–365 (2015).
Otto, F., Yang, Y., Bei, H. & George, E. P. Relative effects of enthalpy and entropy on the phase stability of equiatomic highentropy alloys. Acta Mater. 61, 2628–2638 (2013).
Wang, F. et al. Multiplicity of dislocation pathways in a refractory multiprincipal element alloy. Science 370, 95–101 (2020).
George, E. P., Raabe, D. & Ritchie, R. O. Highentropy alloys. Nat. Rev. Mater. 4, 515–534 (2019).
Miracle, D. B. & Senkov, O. N. A critical review of high entropy alloys and related concepts. Acta Mater. 122, 448–511 (2017).
Maresca, F. & Curtin, W. A. Mechanistic origin of high strength in refractory BCC high entropy alloys up to 1900K. Acta Mater. 182, 235–249 (2020).
Yeh, J.W. et al. Formation of simple crystal structures in CuCoNiCrAlFeTiV alloys with multiprincipal metallic elements. Met. Mater. Trans. A 35, 2533–2536 (2004).
JienWei, Y. E. H. Recent progress in high entropy alloys. Ann. Chim. Sci. Mat. 31, 633–648 (2006).
Rao, S. I., Woodward, C., Akdim, B., Senkov, O. N. & Miracle, D. Theory of solid solution strengthening of BCC chemically complex alloys. Acta Mater. 209, 116758 (2021).
Wen, C. et al. Modeling solid solution strengthening in high entropy alloys using machine learning. Acta Mater. 212, 116917 (2021).
Okamoto, N. L., Yuge, K., Tanaka, K., Inui, H. & George, E. P. Atomic displacement in the CrMnFeCoNi highentropy alloy—a scaling factor to predict solid solution strengthening. AIP Adv. 6, 125008 (2016).
Zhao, Y. Y. & Nieh, T. G. Correlation between lattice distortion and friction stress in Nibased equiatomic alloys. Intermetallics 86, 45–50 (2017).
Zhao, Y. Y., Lei, Z. F., Lu, Z. P., Huang, J. C. & Nieh, T. G. A simplified model connecting lattice distortion with friction stress of Nbbased equiatomic highentropy alloys. Mater. Res. Lett. 7, 340–346 (2019).
Chen, H. et al. Contribution of lattice distortion to solid solution strengthening in a series of refractory high entropy alloys. Met. Mater. Trans. A 49, 772–781 (2018). Phys Metall Mater.
Tong, Y. et al. Severe local lattice distortion in Zrand/or Hfcontaining refractory multiprincipal element alloys. Acta Mater. 183, 172–181 (2020).
Lee, C. et al. Lattice distortion in a strong and ductile refractory highentropy alloy. Acta Mater. 160, 158–172 (2018).
Li, J. et al. Heterogeneous lattice strain strengthening in severely distorted crystalline solids. Proc. Natl Acad. Sci. 119, e2200607119 (2022).
Samolyuk, G. D., Osetsky, Y. N., Stocks, G. M. & Morris, J. R. Role of static displacements in stabilizing body centered cubic high entropy alloys. Phys. Rev. Lett. 126, 025501 (2021).
Ikeda, Y., Gubaev, K., Neugebauer, J., Grabowski, B. & Körmann, F. Chemically induced local lattice distortions versus structural phase transformations in compositionally complex alloys. NPJ Comput. Mater. 7, 1–8 (2021).
Tsai, K. Y., Tsai, M. H. & Yeh, J. W. Sluggish diffusion in co–cr–fe–mn–ni highentropy alloys. Acta Mater. 61, 4887–4897 (2013).
Wang, R. et al. Effect of lattice distortion on the diffusion behavior of highentropy alloys. J. Alloy. Compd. 825, 154099 (2020).
Mu, S., Wimmer, S., Mankovsky, S., Ebert, H. & Stocks, G. M. Influence of local lattice distortions on electrical transport of refractory high entropy alloys. Scr. Mater. 170, 189–194 (2019).
Zhang, Y. et al. Influence of chemical disorder on energy dissipation and defect evolution in concentrated solid solution alloys. Nat. Commun. 6, 1–9 (2015).
Zou, Y., Maiti, S., Steurer, W. & Spolenak, R. Sizedependent plasticity in an Nb25Mo25Ta25W25 refractory highentropy alloy. Acta Mater. 65, 85–97 (2014).
Zunger, A., Wei, S. H., Ferreira, L. G. & Bernard, J. E. Special quasirandom structures. Phys. Rev. Lett. 65, 353 (1990).
Song, H. et al. Local lattice distortion in highentropy alloys. Phys. Rev. Mater. 1, 023404 (2017).
Oh, H. S. et al. Lattice distortions in the FeCoNiCrMn high entropy alloy studied by theory and experiment. Entropy 18, 321 (2016).
Ishibashi, S., Ikeda, Y., Körmann, F., Grabowski, B. & Neugebauer, J. Correlation analysis of strongly fluctuating atomic volumes, charges, and stresses in bodycentered cubic refractory highentropy alloys. Phys. Rev. Mater. 4, 023608 (2020).
Feng, B. & Widom, M. Elastic stability and lattice distortion of refractory high entropy alloys. Mater. Chem. Phys. 210, 309–314 (2018).
Guo, W. et al. Local atomic structure of a highentropy alloy: an Xray and neutron scattering study. Met. Mater. Trans. A Phys. Met. Mater. Sci. 44, 1994–1997 (2013).
Ye, Y. F. et al. Atomicscale distorted lattice in chemically disordered equimolar complex alloys. Acta Mater. 150, 182–194 (2018).
Meng, F. et al. Charge transfer effect on local lattice distortion in a HfNbTiZr high entropy alloy. Scr. Mater. 203, 114104 (2021).
Noehring, W. G. & Curtin, W. A. Correlation of microdistortions with misfit volumes in high entropy alloys. Scr. Mater. 168, 119–123 (2019).
Hu, Y.J., Sundar, A., Ogata, S. & Qi, L. Screening of generalized stacking fault energies, surface energies and intrinsic ductile potency of refractory multicomponent alloys. Acta Mater. 210, 116800 (2021).
Dunitz, J. D., Schomaker, V. & Trueblood, K. N. Interpretation of atomic displacement parameters from diffraction studies of crystals. J. Phys. Chem. 92, 856–867 (1988).
Zhang, F. et al. Chemical complexity induced local structural distortion in NiCoFeMnCr highentropy alloy. Mater. Res. Lett. 6, 450–455 (2018).
Ong, S. P. et al. Python Materials Genomics (pymatgen): a robust, opensource python library for materials analysis. Comput. Mater. Sci. 68, 314–319 (2013).
Liu, J., Zhou, C. & Wang, H. Thermodynamic reoptimizations of the Ru–X (X= Al, Hf, Mo, Ti) binary systems. Calphad 72, 102239 (2021).
Hu, Y.J. et al. Local electronic descriptors for solutedefect interactions in bcc refractory metals. Nat. Commun. 10, 1–11 (2019).
Hartigan, J. A. & Hartigan, P. M. The dip test of unimodality. Ann. Stat. 13, 70–84 (1985).
Li, Z. & Raabe, D. Strong and ductile nonequiatomic highentropy alloys: design, processing, microstructure, and mechanical properties. JOM 69, 2099–2106 (2017).
Ye, Y. X. et al. Evaluating elastic properties of a bodycentered cubic NbHfZrTi highentropy alloy–A direct comparison between experiments and ab initio calculations. Intermetallics 109, 167–173 (2019).
Borg, C. K. H. et al. Expanded dataset of mechanical properties and observed phases of multiprincipal element alloys. Sci. Data 7, 1–6 (2020).
Feuerbacher, M., Heidelmann, M. & Thomas, C. Plastic deformation properties of Zr–Nb–Ti–Ta–Hf highentropy alloys. Philos. Mag. 95, 1221–1232 (2015).
Huang, H. et al. Phase‐transformation ductilization of brittle high‐entropy alloys via metastability engineering. Adv. Mater. 29, 1701678 (2017).
Hu, Y.M. et al. Microstructure and mechanical properties of NbZrTi and NbHfZrTi alloys. Rare Met. 38, 840–847 (2019).
Qiao, D.X. et al. A novel series of refractory highentropy alloys Ti2ZrHf0. 5VNbx with high specific yield strength and good ductility. Acta Met. Sin.ENGL 32, 925–931 (2019).
Maiti, S. & Steurer, W. Structuraldisorder and its effect on mechanical properties in singlephase TaNbHfZr highentropy alloy. Acta Mater. 106, 87–97 (2016).
Coury, F. G., Kaufman, M. & Clarke, A. J. Solidsolution strengthening in refractory high entropy alloys. Acta Mater. 175, 66–81 (2019).
Senkov, O. N., Gorsse, S. & Miracle, D. B. High temperature strength of refractory complex concentrated alloys. Acta Mater. 175, 394–405 (2019).
Fazakas, E. et al. Experimental and theoretical study of Ti20Zr20Hf20Nb20X20 (X= V or Cr) refractory highentropy alloys. Int. J. Refract Hard Met. 47, 131–138 (2014).
Senkov, O. N., Wilks, G. B., Scott, J. M. & Miracle, D. B. Mechanical properties of Nb sub (25 Mo) sub (2) 5 Ta sub (25 W) sub (2) 5 and V sub (20 Nb) sub (2) 0 Mo sub (20 Ta) sub (2) 0 W sub (20 refractory high entropy alloys). Intermetallics 19, 698–706 (2011).
Juan, C.C. et al. Enhanced mechanical properties of HfMoTaTiZr and HfMoNbTaTiZr refractory highentropy alloys. Intermetallics 62, 76–83 (2015).
Guo, N. N. et al. Microstructure and mechanical properties of insitu MCcarbide particulatesreinforced refractory highentropy Mo0. 5NbHf0. 5ZrTi matrix alloy composite. Intermetallics 69, 74–77 (2016).
Han, Z. D. et al. Effect of Ti additions on mechanical properties of NbMoTaW and VNbMoTaW refractory high entropy alloys. Intermetallics 84, 153–157 (2017).
Lin, C.M., Juan, C.C., Chang, C.H., Tsai, C.W. & Yeh, J.W. Effect of Al addition on mechanical properties and microstructure of refractory AlxHfNbTaTiZr alloys. J. Alloy. Compd. 624, 100–107 (2015).
Liu, Y. et al. Microstructure and mechanical properties of refractory HfMo0. 5NbTiV0. 5Six highentropy composites. J. Alloy. Compd. 694, 869–876 (2017).
Yao, H. W. et al. Mechanical properties of refractory highentropy alloys: experiments and modeling. J. Alloy. Compd. 696, 1139–1150 (2017).
Wei, Q. et al. Microstructure evolution, mechanical properties and strengthening mechanism of refractory highentropy alloy matrix composites with addition of TaC. J. Alloy. Compd. 777, 1168–1175 (2019).
Dirras, G. et al. Mechanical behavior and microstructure of Ti20Hf20Zr20Ta20Nb20 highentropy alloy loaded under quasistatic and dynamic compression conditions. Mater. Charact. 111, 106–113 (2016).
Guo, N. N. et al. Microstructure and mechanical properties of refractory MoNbHfZrTi highentropy alloy. Mater. Des. 81, 87–94 (2015).
Wu, Y. D. et al. Phase composition and solid solution strengthening effect in TiZrNbMoV highentropy alloys. Mater. Des. 83, 651–660 (2015).
Wu, Y. D. et al. A refractory Hf25Nb25Ti25Zr25 highentropy alloy with excellent structural stability and tensile properties. Mater. Lett. 130, 277–280 (2014).
Couzinié, J. P. et al. On the room temperature deformation mechanisms of a TiZrHfNbTa refractory highentropy alloy. Mater. Sci. Eng.: A 645, 255–263 (2015).
Dirras, G. et al. Elastic and plastic properties of ascast equimolar TiHfZrTaNb highentropy alloy. Mater. Sci. Eng. A 654, 30–38 (2016).
Yao, H. W. et al. NbTaV(Ti, W) refractory highentropy alloys: experiments and modeling. Mater. Sci. Eng. A 674, 203–211 (2016).
Han, Z. D. et al. Microstructures and mechanical properties of TixNbMoTaW refractory highentropy alloys. Mater. Sci. Eng. A 712, 380–385 (2018).
Chen, S. Y., Yang, X., Dahmen, K. A., Liaw, P. K. & Zhang, Y. Microstructures and crackling noise of AlxNbTiMoV high entropy alloys. Entropy 16, 870–884 (2014).
Yao, H. et al. MoNbTaV mediumentropy alloy. Entropy 18, 189 (2016).
Tseng, K.K. et al. Effects of Mo, Nb, Ta, Ti, and Zr on mechanical properties of equiatomic HfMoNbTaTiZr alloys. Entropy 21, 15 (2018).
Zýka, J. et al. Microstructure and room temperature mechanical properties of different 3 and 4 element medium entropy alloys from HfNbTaTiZr system. Entropy 21, 114 (2019).
Qiao, D. X., Jiang, H., Chang, X. X., Lu, Y. P. & Li, T. J. Microstructure and mechanical properties of VTaTiMoAl_{x} refractory high entropy alloys. Mater. Sci. Forum 898, 638–642 (2017).
Guo, N. N. et al. Effect of composing element on microstructure and mechanical properties in Mo–Nb–Hf–Zr–Ti multiprinciple component alloys. Intermetallics 69, 13–20 (2016).
Varvenne, C., Leyson, G. P. M., Ghazisaeidi, M. & Curtin, W. A. Solute strengthening in random alloys. Acta Mater. 124, 660–683 (2017).
Vegard, L. Die konstitution der mischkristalle und die raumfüllung der atome. Z. für. Phys. 5, 17–26 (1921).
Noble, B., Harris, S. J. & Dinsdale, K. The elastic modulus of aluminiumlithium alloys. J. Mater. Sci. 17, 461–468 (1982).
Andersson, J.O., Helander, T., Höglund, L., Shi, P. & Sundman, B. ThermoCalc & DICTRA, computational tools for materials science. Calphad 26, 273–312 (2002).
Owen, L. R. & Jones, N. G. Lattice distortions in highentropy alloys. J. Mater. Res. 33, 2954–2969 (2018).
Welch, B. L. The generalization of ‘STUDENT’S’ problem when several different population varlances are involved. Biometrika 34, 28–35 (1947).
Sutton, A. P., Finnis, M. W., Pettifor, D. G. & Ohta, Y. The tightbinding bond model. J. Phys. C: Solid State Phys. 21, 35 (1988).
Tandoc, C. & Hu, Y.J. A bond counting model Using B2 intermetallic calculations for efficient estimation of BCC MPEA lattice parameter with superior accuracy. arXiv preprint at https://doi.org/10.48550/arXiv.2203.07137 (2022).
Rice, J. R. Dislocation nucleation from a crack tip: an analysis based on the Peierls concept. J. Mech. Phys. Solids 40, 239–271 (1992).
Yang, X., Zhang, Y. & Liaw, B. Microstructure and compression properties of highentropy alloys NbTiVTaAl x. Procedia Eng. 36, 292–298 (2012).
Huang, H. et al. On cooling rates dependence of microstructure and mechanical properties of refractory highentropy alloys HfTaTiZr and HfNbTiZr. Scr. Mater. 211, 114506 (2022).
Blöchl, P. E. Projector augmentedwave method. Phys. Rev. B 50, 17953 (1994).
Perdew, J. P., Burke, K. & Ernzerhof, M. Generalized gradient approximation made simple. Phys. Rev. Lett. 77, 3865 (1996).
Kresse, G. & Furthmüller, J. Efficient iterative schemes for ab initio totalenergy calculations using a planewave basis set. Phys. Rev. B 54, 11169 (1996).
Körmann, F., Ikeda, Y., Grabowski, B. & Sluiter, M. H. Phonon broadening in high entropy alloys. NPJ Comput. Mater. 3, 1–9 (2017).
Clouet, E., Nastar, M. & Sigli, C. Nucleation of Al 3 Zr and Al 3 Sc in aluminum alloys: From kinetic Monte Carlo simulations to classical theory. Phys. Rev. B 69, 064109 (2004).
Shu, S., Wells, P. B., Almirall, N., Odette, G. R. & Morgan, D. D. Thermodynamics and kinetics of coreshell versus appendage coprecipitation morphologies: an example in the FeCuMnNiSi system. Acta Mater. 157, 298–306 (2018).
Acknowledgements
C.T. and Y.J.H. thank the financial support from the startup fund from Drexel University. L.Q. acknowledge the financial support from the National Science Foundation (NSF) Award DMR1847837. P.K.L. very much appreciates the supports from (1) the National Science Foundation (DMR1611180, 1809640, and 2226508) and (2) the US Army Research Office (W911NF13–10438 and W911NF19–20049). The computational support from the Drexel’s University Research Computing Facility is greatly acknowledged. A part of the calculations was also carried out using the Extreme Science and Engineering Discovery Environment (XSEDE) Stampede2 at the TACC through allocation TGDMR190035, and allocation MAT220033 from the Advanced Cyberinfrastructure Coordination Ecosystem: Services & Support (ACCESS) program, which is supported by National Science Foundation Grants #2138259, #2138286, #2138307, #2137603, and #2138296.
Author information
Authors and Affiliations
Contributions
Y.J.H. conceptualized and supervised the research project. C.T. performed the firstprinciples calculations, development of descriptors and statistical learning models, and data mining of alloy properties. C.T., Y.J.H., L.Q., and P.K.L. prepared the manuscript. All authors discussed the results and contributed to the manuscript.
Corresponding author
Ethics declarations
Competing interests
The authors declare no competing interests.
Additional information
Publisher’s note Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
Supplementary information
Rights and permissions
Open Access This article is licensed under a Creative Commons Attribution 4.0 International License, which permits use, sharing, adaptation, distribution and reproduction in any medium or format, as long as you give appropriate credit to the original author(s) and the source, provide a link to the Creative Commons license, and indicate if changes were made. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in a credit line to the material. If material is not included in the article’s Creative Commons license and your intended use is not permitted by statutory regulation or exceeds the permitted use, you will need to obtain permission directly from the copyright holder. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/.
About this article
Cite this article
Tandoc, C., Hu, YJ., Qi, L. et al. Mining of lattice distortion, strength, and intrinsic ductility of refractory high entropy alloys. npj Comput Mater 9, 53 (2023). https://doi.org/10.1038/s4152402300993x
Received:
Accepted:
Published:
DOI: https://doi.org/10.1038/s4152402300993x
This article is cited by

Microstructure Design of Multiphase Compositionally Complex Alloys II: Use of a Genetic Algorithm and a Vanishing Cracked Particle Model
High Entropy Alloys & Materials (2024)